houghton on quenching
Post on 22-Nov-2014
Embed Size (px)
CONTENTSINTRODUCTION THE FUNDAMENTALS OF QUENCHING THE MECHANISM OF QUENCHING WATER AND SALT SOLUTIONS QUENCHING OILS POLYMER QUENCHANTS QUENCHING SYSTEM DESIGN QUENCHANT SELECTION QUENCHING PROBLEMS AND THEIR CAUSES SUMMARY 2 3 7 11 15 23 46 54 60 74
INTRODUCTIONThe Houghton organization is a worldwide leader in heat treatment, supplying quenching fluids and associated products, technology and application expertise across a wide range of industries. Quenching has, for a long time, been regarded as a black art, surrounded by fumes, fire, mystery and intrigue. Although the quenching process takes only a few seconds of the total production time for a component - which can be as long as six months or more from the start of Oil quenching of critical aerospace manufacture to the shipment of the finished components product - it is often neglected or considered a low priority. Lack of understanding of the principles and practices of quenching can result in inadequate hardness, excessive distortion or scrapping of costly machined components, together with the environmental problems of smoke, fumes and fire hazards frequently associated with the heat treatment shop. These web pages are designed to dispel the mystery surrounding the quenching process and give guidance for the selection of quenchants and the design of a quenching system so that improved performance, greater efficiency and maximum safety can be obtained.Heat Treatment of alloy steel bars
Fire Hazard during oil quenching
After conversion to Aqua-Quench polymer quenchant
THE FUNDAMENTALS OF QUENCHINGHeat treatment can be defined as an operation or combination of operations involving the controlled heating and cooling of a metal in the solid state for the purpose of obtaining specific properties. There are many types of heattreating process available fulfilling a wide variety of hardness and mechanical properties requirements. This booklet is concerned with the principles and practices of the quenching process. Quenching of steel involves the rapid cooling of austenite to transform it into the hard structure - martensite. This is generally achieved by cooling at a sufficiently fast rate to avoid the formation of soft constituents in the steel (pearlite and bainite). These reactions can be represented on a Continuous Cooling Transformation (CCT) diagram (Figure 1).
Figure 1. Continuous Cooling Transformation diagram illustrating the critical cooling rate for complete martensitic transformation
For a given steel composition and heat treatment condition, there is a critical cooling rate for full hardening at which all the high temperature austenite is transformed into martensite without the formation of either pearlite or bainite. The steel begins to transform at the Ms temperature and is fully hardened at the Mf temperature. The Ms temperature decreases with increasing carbon content of the steel as shown below:
Ms Temperature as a function of carbon content Carbon Content Ms Temperature
0.2% 0.4% 1.0%
430C 360C 250C
In practice, however, when a steel component is quenched, the surface cools more rapidly than the center. This means that the surface could cool at the critical cooling rate and hence be fully hardened, whereas the center cools more slowly and forms soft pearlitic or bainitic structures (Figure 2).
Figure 2. The effect of component section thickness on cooling rate.
Lack of through hardening can be overcome by one of two methods. By increasing the hardenability of the component by the use of an alloy with higher alloy content. This usually causes a delay in transformation, illustrated by a shift to the right in the CCT diagram. This reduces the critical cooling rate for martensitic transformation producing fully hardened components with maximum hardness and mechanical properties (Fig. 3). Alloying elements can, however, be expensive and may not be beneficial to other processes, i.e., machining, forging, etc.
Fig. 3. The effect of alloy content on steel hardenability.
By increasing the quenching speed so that the cooling rate at the center of the component exceeds the critical cooling rate. This can be achieved, for example, by changing from a normal speed quenching oil to a high speed accelerated quenching oil (Fig. 4) or, if using a polymer quenchant, by reducing the concentration of the solution.
Fig. 4. The effect of quenching speed on hardness and mechanical properties.
The influence of quenching speed on hardness and mechanical properties can be illustrated by comparing the cross-sectional hardnesses achieved in a 10 mm diameter bar of 0.4% carbon steel quenched into different types of oil (Fig. 5). With normal speed oil, hardness decreases rapidly below the surface due to the formation of pearlite and bainite. With highspeed oil, the critical cooling rate is exceeded to a much greater depth below the surface, resulting in an improved hardness profile.
Fig. 5. The effect of quenching oil type on cross-sectional hardness
To summarize therefore, steel composition, component section thickness, and type of quenchant all have a major influence on the properties obtained in the heat-treated component.
THE MECHANISM OF QUENCHINGIt is important to understand the mechanism of quenching and the factors, which affect it, since these can have a significant influence on quenchant selection and the performance obtained from the quenching process. Regardless of the type of quenchant being used, cooling generally occurs in three distinct stages, each of which has very different characteristics (Fig. 6).
Fig. 6 The three stages of cooling during quenching Stage 1. Vapor Phase Stage 2. Boiling Phase Stage 3. Convection Phase
The first stage of cooling is characterized by the formation of a vapor film around the component. This is a period of relatively slow cooling which heat transfer occurs by radiation and conduction through the vapor blanket.
The stable vapor film eventually collapses and cool quenchant comes into contact with the hot metal surface resulting in nucleate boiling and high heat extraction rates.
Boiling ceases and heat is removed by convection into the liquid. Heat is removed very slowly during this stage
Fig. 7. This series of photographs illustrates the various stages in the quenching process using a normal speed quenching oil.
The moment of immersion - After 5 seconds - boiling After 10 seconds - the boiling vapor film around component commences at the corners of front moves along the (stage 1). the component (stage 2). component.
After 15 seconds - showing After 30 seconds - convection After 60 seconds - completion vapor, boiling and convection phase (stage 3). of convection phase. phases.
The cooling characteristics of a quenchant can be measured using probes instrumented with thermocouples. Various techniques have been used including both cylindrical and spherical probes manufactured from a variety of metals including stainless steel, silver and nickel alloys. One of the most widely used and accepted methods is based upon the use of a 12.5 mm diameter cylindrical probe manufactured from Inconel 600 alloy as 8
specified in the Wolfson Heat Treatment Center (WHTC) Engineering Group specification recommended by the International Federation for Heat Treatment (IFHT) and adopted by the International Standards Organization (ISO 9950). Results obtained by the different test methods vary depending upon the material, geometry and surface condition of the probe. Cooling curves produced in this way illustrate well the three stages of quenching and demonstrate the influence that factors such as agitation, quenchant temperature, contamination and degradation have upon quenching performance. The cooling characteristics can either be shown as a graph of temperature against time or as a graph of temperature against cooling rate as shown in Fig. 8 for both normal speed and high speed quenching oils.
Fig. 8. Temperature-time cooling curve and differential cooling curve
Such cooling curve information is valuable since it can theoretically be superimposed upon CCT diagrams to predict heat-treatment response (Figure 9). The duration of the vapor phase and the temperature at which the maximum cooling rate occurs have a critical influence on the ability of the steel to harden fully. The rate of cooling in the convection phase is also important since it is generally within this temperature range that martensitic transformation occurs and it can, therefore, influence residual stress, distortion and cracking. However, cooling curves produced under laboratory conditions must be interpreted carefully and should not be considered in isolation. Results on 9
used quenchants should be compared with reference curves for the same fluid.
Fig. 10. The effect of on the Fig. 9. Temperature-time cooling curve on CCT agitation quenching characteristics diagram. of a normal speed oil.
Quenching characteristics are influenced significantly by the degree of agitation, as shown in Fig. 10 for a normal speed quench oil under varying degrees of propeller agitation. It can be seen that increasing the degree of agitation reduces the stability of the vapor phase and increases the maximum rate of cooling. The performance obtained from a quenchant in practice, therefore, depends upon actual conditions Fig. 11. ivf quenchotest. in the quench tank. For this reason, it is highly desirable to measure quenching characteristics on site. Specialized, fully portable and self-contained equipment has been developed for this purpose by IVF (The Swedish Institute of Production Engineering Research) (Fig. 11). This equipment conforms to widely accepted industrial stan